10.6092/issn.1973-9494/1246
The patina represents a superficial natural alteration of the constituting matter of the work of art. It emerges from the natural and usual stabilization process that the materials of the surface undergo because of the interaction with outdoor agents characterizing the surrounding environment. Besides, it is not linked to an obvious phenomenon of degradation that can be noticed through the change in the original colour of the matter.
This is what we intend when we talk about biological patina usually generated by macro and/or micro-organic colonization (fungi, bacteria, alga) which contributes to surface bio-deterioration and thus lead to the formation of orange, red or even brown and dark pigmented areas. The presence of chromatic alterations (rose-coloured areas), as a consequence of bacterial colonization, was most particularly pointed out in different sites, such as in the marble slabs on the facades of both the Cathedral of Siena (Duomo di Siena) and the Certosa of Pavia. The present study shows an example of chromatic alteration of the surface of marble works due to bacterial colonization.
application/pdf
1973-9494
1246
en
Laura Ercoli
Conservation Science in Cultural Heritage
Assessment of the conservation state of stone materials in relation to the level environmental pollution in the conservation place
Text.Serial.Journal
https://conservation-science.unibo.it/
7
Articles
2008-07-07
2007-07-08
2015-11-02
CSCH
Laura Ercoli
2007
10.6092/issn.1973-9494/1246
1973-9494
en
Assessment of the conservation state of stone materials in relation to the level environmental pollution in the conservation place
https://conservation-science.unibo.it/article/download/1246/670
7
A
    SSESMENT OF THE CONSERVATION STATE
    OF STONE MATERIALS IN RELATION TO THE LEVEL
    ENVIRONMENTAL POLLUTION IN THE CONSERVATION PLACE

Giovanni Rizzo, Fabio D’Agostino, Bartolomeo Megna, Maria Parlapiano
Dipartimento di Ingegneria Chimica dei Processi e dei Materiali
Università degli Studi di Palermo
Laura Ercoli
Dipartimento di Ingegneria Strutturale e Geotecnica
Università degli Studi di Palermo




1. Introduction

    In the last decades, the environmental conditions of exposure of the cultural heritage
– many of them to be found in urban areas –, have gradually become more aggressive,
causing an acceleration of the degradation process and sometimes jeopardizing the
results of interventions aiming at the preservation of surfaces [1-2]. One of the main caus-
es may be linked to the uncontrolled increase of the traffic. If we don’t consider the impor-
tance of the cultural heritage, there seems to be no real possibility of limitations so as to
protect monuments, neither to preserve the health of citizens living in urban centres.


                                                                                                  Conservation Science in Cultural Heritage# $/!%%$
However, the enforced regulations in the field of protection of the public health indicates
the concentration limits of atmospheric pollutants. If these limits are exceeded, the Local
Authorities must intervene to restore security conditions. A similar approach would be
advisable for the preservation of the cultural heritage with a quantification of the relative
pollution risks which aims at developing legislative and operative interventions useful to
reduce the presence of aggressive components in areas with a high historical-artistic
content, as it is the case in the historical centre of Palermo.
    The long term project SALVALARTE Respira Pulito has been recently promoted by
the Agenzia Regionale per la Protezione Ambientale (A.R.P.A.), by the Centro Regionale
per la Progettazione e il Restauro (C.R.P.R.) of the Assessorato Beni Culturali della
Regione Sicilia, by Legambiente and by a number of research groups of the three uni-
versities operating in Sicily. This is a multidisciplinary research project [3] which provides
in a first stage data collection concerning the conservation state of the cultural heritage
in Sicily, and which contributes to the definition of a “cultural heritage risks card” that is

                                                                                                 !"
                                                                                                            under creation by the C.R.P.R. and that also regards the preservation in indoor locations
                                                                                                            [4]. One of the relevant aspects of the research, in relation to the wide spectrum of com-
                                                                                                            petences of the involved subjects, is to assess both the different causes of alteration,
                                                                                                            starting from chemical causes to physical or biological ones, and to measure the most
                                                                                                            important environmental chemical-physical parameters so as to link them with the con-
                                                                                                            servation state of monuments [5-6].
                                                                                                                The first part of the research was executed in Palermo along Vittorio Emanuele
                                                                                                            Avenue that crosses the historical centre of the city from the mountains down to the sea
                                                                                                            and is characterised by an important traffic. The duty of the Laboratory of Chemical
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                            Engineering for Cultural Heritage, University of Palermo, is emphasized in the following
                                                                                                            points:
                                                                                                            –   analysis for the characterisation of the most recurrent constitutive materials of histor-
                                                                                                                ical-artistic works (construction and facing stones, gypsums, stucco, (non) structural
                                                                                                                wood, bricks, etc.);
                                                                                                            –   measure of the chemical-physical parameters that define their conservation state;
                                                                                                            –   analysis of samples of particles gathered by the Municipal concern of environmental
                                                                                                                Health (A.M.I.A.) and by the ARPA Sicily;
                                                                                                            –   analysis of the causes and of the mechanisms of the alteration and degradation
                                                                                                                process of the materials and correlation with the exposure conditions, defined by
                                                                                                                means of environmental monitoring carried out by the other groups of research.
                                                                                                                In this paper the results of a first sampling campaign organized with the other part-
                                                                                                            ners of the project are displayed.

                                                                                                            2. Materials and experimental techniques

                                                                                                                The art works in which the research is interested are the two monumental gates that
                                                                                                            bound Vittorio Emanuele Avenue, i.e Porta Nuova on the upper side and Porta Felice
                                                                                                            down on the sea side, and the Biblioteca Centrale della Regione Sicilia (we will refer to it
                                                                                                            in this paper as Central Library of the Sicilian Region) that overlooks the middle of the
                                                                                                            avenue.
                                                                                                                For each building, a photographic campaign was carried out to know the different typolo-
                                                                                                            gies of degradation. For each collected sample, a form containing the photograph and the
                                                                                                            description of the surveyed area was filled out. In the areas where it was not possible to
                                                                                                            take a sample, the phenomena of degradation were described by direct observation.
                                                                                                                The typology of the sampled materials includes natural stones, mortars, crusts, super-
                                                                                                            ficial deposits and saline efflorescence. The sampling was always carried out with non

                                                                                                       &%
invasive techniques, collecting the material in secluded or not accessible zones and try-
ing to keep close to the monitoring point chosen by the other groups. Furthermore,
numerous samples of atmospheric particles were analysed, because their composition in
terms of crystalline species, heavy metal and soluble salts may highly influence the dura-
bility of stony materials. The samples of particles were collected both by the A.M.I.A. mon-
itoring stations, the office that has the duty to collect the particles and quantify their pres-
ence in the air, and by two monitoring campaigns of the air quality carried out by ARPA
Sicily in the Central Library and in the Regional Archaeological Museum A. Salinas. The
collected dusts were then analysed by the Laboratorio di Ingegneria Chimica for Cultural
Heritage, in collaboration with the Provincial Department (DiP) of Palermo of the ARPA
Sicily.
    After microscopic observation of the sample, the chosen analytical techniques are X-
ray diffractometry (XRD), ionic chromatography (IC), emission spectrophotometry with
plasma source, mass spectrometry (ICP-MS) carried out by the DiP of the ARPA.

3. Results and remarks

    In the following tables, the analytical results are reported and presented according to
the specific origin of the sample and to the typology of analysis. Both for the Central
Library of the Sicilian Region and for Porta Felice, ten samples composed of crusts, mor-
tars and saline efflorescence were analysed (tab. 1-3). As regards Porta Nuova, a wide
campaign of sampling was carried out, in the frame of restoration interventions made in
2000, on both the façades, the results of which were published [7]. In this paper, the char-
acteristics of only two samples collected in the frame of the project SALVALARTE respi-
ra pulito (tab. 4-5) are showed as an example.
                                                                                                       Conservation Science in Cultural Heritage


    The results of the XRD analysis reported in tab. 2 show that the gypsum is present
only in the samples referred to as “croste”. The origin of gypsum can be linked to a sul-
phation process of carbonate substratum, as an example marbles and calcareous stones,
but also mortars based on lime. Nevertheless, the XRD analysis reported in tab. 6 shows
the presence of gypsum in atmospheric particles too, as a consequence of the Aeolian
dragging from gypsiferous soils. As a consequence, some of the samples called “croste”
could actually be the result of the consolidation of a deposit of particles onto the stony
surfaces. This topic of the conservation state of the buildings will be analysed thorough-
ly with the help of the other operative unities of the project SALVALARTE respira pulito
that has the aim of detecting the gas components of the urban atmosphere, and in par-
ticular SO2.

                                                                                                   &
                                                                                                                Table 1. Results of the XRD analysis on samples coming from the Central
                                                                                                                Library of the Sicilian Region. The symbols + show the relative abundance.




                                                                                                                                                                                                                                                                             hexahydrite
                                                                                                                                                                                                                                                    soda niter
                                                                                                                                                                 dolomite


                                                                                                                                                                             Gypsum
                                                                                                                                                      calcite




                                                                                                                                                                                           quartz


                                                                                                                                                                                                                 halite


                                                                                                                                                                                                                              niter
                                                                                                                  Sample
                                                                                                                  Library 01 salt                     +                     +++
                                                                                                                  Library 02 sali                                                                         +++                 +                sign
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                                  Library 03 “crosta”              ++           sign        +             sign
                                                                                                                  Library 04 salt                  ++                       +             ++                                                                                 +
                                                                                                                  Library 05 mortar                ++                       +
                                                                                                                  Library 06 cement                   +         sign                       +
                                                                                                                  Library 07 “crosta”              ++           +++         +              +
                                                                                                                  Library 08 deposit               ++           ++                         +
                                                                                                                  Library 09 mortar                ++           ++                         +
                                                                                                                  Library 12 salt                  ++            +



                                                                                                            Table 2. Results of the XRD analysis on samples coming from Porta Felice.
                                                                                                                                                                                                                                      Hexahydrite




                                                                                                                                                                                                                                                                                                                     Thenardite
                                                                                                                                                                                                                                                                                           “Glauber’s
                                                                                                                                                                                                     Muscovite




                                                                                                                                                                                                                                                                                                         Picromite
                                                                                                                                                                                                                                                                                            Mirabilite
                                                                                                                                               Dolomite




                                                                                                                                                                                                                                                                  Feldspar
                                                                                                                                                                 Gypsum
                                                                                                                                    Calcite




                                                                                                                                                                                 Quartz




                                                                                                                                                                                                                          Niter




                                                                                                                                                                                                                                                                                              salt”




                                                                                                             PF 01 “crosta”     +++                              +               +
                                                                                                             PF 02 “crosta”                                     ++               +
                                                                                                             PF 03 salt         +++           sign                                                                                    +
                                                                                                             PF 04 salt         +++                                                                                       +           ++
                                                                                                             PF 05 “crosta”         +                           ++           sign
                                                                                                             PF 07 “crosta”         +         ++++                               +                                                                               sign
                                                                                                             PF 08 plaster      +++           ++++                           sign                   sign
                                                                                                             PF 09 salt                                                                                                               +                                                      +++         +
                                                                                                             PF 10 salt                                                                                                                                                                      +++         +           +
                                                                                                             PF 11 salt         ++             +


                                                                                                       &!
Table 3. Results of the analysis by ionic chromatography on samples coming from
Porta Felice (values expressed in % in weight).

                                 Anions                                              Cations




                                              HPO42-


                                                        SO42-




                                                                              NH4+




                                                                                                          Mg2+
                                   NO3-




                                                                                                  Ca2+
                                                                 Na+
                         Cl-




                                                                                       K+
                  F-




    PF 02        0.01   0.14      0.05                 24.6     0.22                  0.12       12.45   0.04

    PF 03        0.01   0.54      0.09                 12.07    0.21                  0.44       0.67    3.83

    PF 04        0.01   0.18      0.23                 15.39    0.53                  0.17       0.81    3.99

    PF 07        0.01   0.39                           0.20     0.28      0.07        0.08       1.15    0.21

    PF 08        0.01   0.13      0.05                 24.53    2.01                  0.18       0.42    0.06

    PF 09               0.07      0.03                 24.68    8.59                  8.47       0.69    2.22

    PF 10        0.01   0.15      0.07       0.11      24.45    16.43                0,0625      0.43    0.06
    PF 11        0.02   0.05      0.08                 2.93     0.44                  0.11       1.11    0.63




             Table 4. Results of the XRD analysis on samples coming from Porta
             Nuova.

                                          Calcite      Gypsum           Quartz         Dolomite

                 PN 01 “Crosta”            +++              +            sign
                 PN 02 Deposit              ++           sign             +                 ++
                                                                                                                  Conservation Science in Cultural Heritage



   The presence of either a fair quantity of sodium and magnesium, or chloride and sul-
phate, as showed in tab. 3 and 5, reveals the very important role of marine aerosol to
establish the diffuse presence of saline efflorescence.
   The task of the Laboratory of Chemical Engineering for Cultural Heritage is to assess
the conservation state of the materials. However, considering the multidisciplinary vision
that was adopted, it was thought useful to include the data collected by the other oper-
ative unities concerning the role of outdoor material and the presence of aggressive
compounds in the atmosphere, through the analysis of the atmospheric particles by
means of the same techniques used to characterize the constitutive materials of the
buildings.

                                                                                                                 &&
                                                                                                            Table 5. Results of the chro-                 The samples of particles collected by the
                                                                                                            matographic analysis on 1 sam-             A.M.I.A. come from three monitoring stations,
                                                                                                            ple coming from Porta Nuova.
                                                                                                                                                       respectively located at the end of the Avenue, exact-

                                                                                                                             PN02
                                                                                                                                                       ly at Piazza Indipendenza (I) near Porta Nuova, at
                                                                                                                                                       Piazza Giulio Cesare (G) near the central station of
                                                                                                                  Anions            Weight %
                                                                                                                                                       Palermo where there is very much traffic, and in a
                                                                                                                    F-                0.05
                                                                                                                                                       suburban area of Palermo, Boccadifalco (F), with a
                                                                                                                    Cl-               0.73
                                                                                                                                                       low traffic flow. Two other parameters of great
                                                                                                                   NO3-               0.57
                                                                                                                                                       importance for their influence on the composition of
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                                  Cations
                                                                                                                                                       the atmospheric particles were considered in the
                                                                                                                   Na+                0.38
                                                                                                                                                       classification of the samples: the periods of rainfall
                                                                                                                   NH4+               0.02
                                                                                                                                                       and periods of artificial heating. The samples are
                                                                                                                    K+                0.18
                                                                                                                                                       identified by a first letter that indicates the monitor-
                                                                                                                   Ca2+               1.48             ing station of origin, a second letter that indicates
                                                                                                                   Mg2+               0.26             the presence or not of heating – R for heating and
                                                                                                                                                       N without heating –, a third letter to indicate if the
                                                                                                            sample was collected in a rainy (P) or dry period (S), and finally a progressive number to
                                                                                                            be able to differentiate subsequent samples with the same origin.
                                                                                                               As an example, the sample GRP1 is the first one (1) taken in the monitoring station
                                                                                                            of Giulio Cesare, in a period of heating (R) and rain (P).




                                                                                                                Table 6. Results of the XRD analysis on samples of atmospheric particle col-
                                                                                                                lected by A.M.I.A.

                                                                                                                  Mineralogical phase        Calcite     Dolomite      Quartz      Gypsum       Halite
                                                                                                                           GNS1                ++++         ++           ++           +           +
                                                                                                                           GNS2                ++++         ++           ++           +           +
                                                                                                                            INS1               ++++         ++          +++          ++           ++
                                                                                                                            INS2               ++++         ++          +++           +           ++
                                                                                                                            FNS1               +++          ++           ++           +           +
                                                                                                                            FNS2               +++         +++          +++          ++           ++
                                                                                                                           GRP1                ++++        +++           ++          sign         +
                                                                                                                           GRP2                ++++        +++           ++          sign         +
                                                                                                                            IRP1               ++++         ++          +++           +          +++
                                                                                                                            IRP2               ++++        +++           ++          ++          +++

                                                                                                       &)
 Table 7. Results of the I.C. analysis on samples of atmospheric particle collected by
 A.M.I.A.

                                   Anions [weight %]                                                                 Cations [weight %]




                                                                                   HPO42-



                                                                                                 SO42-




                                                                                                                    NH4+




                                                                                                                                                      Mg2+
                                                  NO2-



                                                                  NO3-




                                                                                                                                         Ca2+
                                                                                                           Na+
                                   Cl-




                                                                                                                                 K+
                      F-




    GNS1             0,02         1,08           0,38            1,6          Sign            2,99        0,85                 0,21    2,69          0,26
    GNS2             0,01         1,5            0,36            2,04         Sign            4,06         0,9                  0,2    3,31          0,28
       INS1          0,01         0,71           0,4             1,13                          4,5        0,73                 0,23    3,23          0,25
       INS2          Sign         1,23           0,3             1,7                          3,87        0,98                 0,19    3,08          0,24
       FNS1          Sign         1,61           Sign            1,03         0,03            5,24        0,82    Sign         0,25    3,93          0,25
       FNS2          0,07         1,67           Sign            2,8          Sign            5,37        1,28                 0,19    3,87          0,28
    GRP1             0,02         2,57           0,01            1,09                         1,58        0,87    Sign         0,14     3,2          0,23
    GRP2             0,02         1,47           0,02            1,39                         1,82        0,99     0,1         0,16    3,31          0,25
       IRP1          Sign         1,44           0,01            0,53                         1,31        0,84    0,03         0,09    2,28          0,14
       IRP2          Sign         1,42           Sign            1,3                          2,97        1,13    Sign         0,15    2,95          0,2


                                         Anions [weight %]                                                               Cations [weight %]
                                                                          HPO42-




                                                                                             SO42-




                                                                                                                  NH4+




                                                                                                                                                             Mg2+
                                          NO2-



                                                          NO3-




                                                                                                                                              Ca2+
                                                                                                          Na+
                            -




                                                                                                                                K+
               F-



                            Cl




FRP1                    10,38            Sign            3,03            Sign               9,23         9,54    Sign          0,33      10,1           1,02
FRP2                       9,91          0,22            3,61                               8,91         9,91    0,7           0,23      12,55          1,02
GRS1                        2,5          0,15            2,04                               3,83         2,07    0,69          0,32      5,95           0,44
GRS2          0,06         1,67          0,09            2,68                               4,85         2,06    Sign          0,09      4,79           0,29
 IRS1         Sign         3,99          0,12            2,06            Sign               6,02         3,72                            5,06           0,65
 IRS2                      7,18          0,2             3,14                               7,64         6,62    0,26          0,25      7,23           0,89
FRS1                       3,18          0,1             2,88                               10,92        3,89    1,57           0,4      5,09           0,78
FRS2                    10,13            0,15            4,35                               9,69         8,52    0,47           0,3      5,77           1,12
 GNP          0,06         1,48          0,09            2,3                                3,74         2,29    0,2           0,18      8,25           0,33
                                                                                                                                                                     Conservation Science in Cultural Heritage

 INP                       1,61          0,15            2,93                               6,54         3,44                  Sign      12,89          0,49




   The results of the XRD, LC and IPC-MS analysis are showed in tab. 7-9.
   The presence of an important quantity of calcite and gypsum in the particles was high-
lighted by the XRD analyses reported in tab. 6 and could be the origin of the consolida-
tion phenomenon of the superficial deposit, as the result of a solubilization and recrys-
tallization process deriving from usual cycles of environmental humidity. This point had
already been emphasized in the frame of a research carried out in collaboration with the
Centre Gino Bozza of the Consiglio Nazionale delle Ricerche of Milano for the town hall
of Palermo [8].

                                                                                                                                                                    &*
                                                                                                            Table 8. Results of the ICP-MS analysis on samples of atmospheric particle collected by
                                                                                                            A.M.I.A.

                                                                                                                                           Macro elements concentration in the atmosphere [ng/Nm3]
                                                                                                                                                     Ca          Mg            Fe            P           Al
                                                                                                                                     GNS          2990           363          598            0           152
                                                                                                                                     INS          3350           396          413            9           157
                                                                                                                                     FNS          3380           523          339           266          184
                                                                                                                                     GRP          7540           1040         942           32           240
                                                                                                                                     IRP          3450           529          553           275          191
                                                                                                                                     FRP          1800           298          140           238          279
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                                                     GRS          7590           912         1000           25           253
                                                                                                                                     IRS          5080           647          622           18           234
                                                                                                                                     FRS          1390           298          121            4           126
                                                                                                                                     GNP          4810           678          864           1010         279
                                                                                                                                     INP          3550           468          465           511          232


                                                                                                                                           Micro elements concentration in the atmosphere [ng/Nm3]
                                                                                                                      Ba      Cd      Cr        Cu        Pb      Mn     Ti          Co          Sb     Sn      V      Zn     Ni
                                                                                                             GNS      17,7   0,147    22,2      173       33      8,04   3          0,338     7,11     2,53    3,99    136    5,11
                                                                                                             INS      12,4   0,029    22,4     20,9       29,5    8,05   3          0,497        3,5   0,963   5,85    87,5   7,43
                                                                                                             FNS      8,91   0,123    19,8     25,1       15,7    9,57   3,5        0,403     13,1     1,20    14,2    18,7   8,69
                                                                                                             GRP      32,8   0,156    27,6     52,9       56,2    12,3   4,9        0,611     11,5     2,83    1,63    59,7   5,32
                                                                                                             IRP      18,9   0,159    20,2     32,0       43      8,5    2,6        0,207     7,96     1,46    1,28    39     6,26
                                                                                                             FRP      4,39   0,014    16,1     11,9       4,74    3,47   5,2        0,236     1,84     0,222   0,714   8,38   9,35
                                                                                                             GRS      30,5   0,154    28,3     54,9       62,8    12,8   5,1        0,449     13,1     2,71    3,58    84,2   17,4
                                                                                                             IRS      18,3   0,208    26,3     34,5       50,3    8,82   2,7        0,332        8,2   1,98    2,90    74,1   5,55
                                                                                                             FRS      4,49   0,018    26,9      6,3       7,25    2,39   5,1        0,197    0,815     0,452   1,34    11,8   6,30
                                                                                                             GNP      17,9   0,361    4,57      53        36,7     11    4,6        0,445     12,9     0,550   3,85    33,3   6,35
                                                                                                             INP      13,8   0,097    14,8     24,8       31,5    7,28   3,8        0,220     5,22     0,348   3,51    24,1   12,5




                                                                                                                   A comparison drawn between the results of the A.M.I.A. analysis on filters and those
                                                                                                            of the ARPA displays a particular critical state of the Central Library that overlooks on the
                                                                                                            narrow Vittorio Emanuele Avenue. That state is indeed worse than in two squares, Piazza
                                                                                                            Giulio Cesare and Piazza Indipendenza place, that bear a high traffic flow and that are
                                                                                                            not located that far from the Central Library. In particular, the concentration of macro ele-
                                                                                                            ments of the samples BC reported in tab. 9 appears, in many cases, higher, even by
                                                                                                            order of size, than for the samples G and I of tab. 8. This result shows the presence of a
                                                                                                            greater quantity of atmospheric particles near the Library, probably as a consequence of
                                                                                                            the so-called “canyon effect” that contributes to trapping pollutants, with a particular ref-
                                                                                                            erence to those emitted by vehicles at a low quote in the city. This very phenomenon is

                                                                                                       &+
Table 9. Results of the ICP-MS analysis on samples of atmospheric particle collected by
ARPA Sicily near the Archaeological Museum of Palermo (MA) and the Central Library of
Sicilian Region.

                             Macro elements concentration in the atmosphere [ng/Nm3]
                                      Ca            Mg              Fe              Al
                            MA1       770           270           <L.R.             70
                            MA2      1720           190            190              220
                            MA3      2380           440            420              530
                            BC1      7750           1520           1020             350
                            BC2      11600          2190           1120             460


                             Micro elements concentration in the atmosphere [ng/Nm3]

       B     Ba      Cd       Co      Cr     Cu       Mn    Ni     Pb      S       Sb      Sn      Ti      V     Zn
 MA1   3     5,9     0,5     <L.R.   <L.R.   7,8      1,4   5,3   <L.R.   <L.R.   <L.R.    9,5    <L.R.   0,3    7,4
 MA2   3,3   9,4     0,2     <L.R.   <L.R.   9,4      2,3   1      5,9    <L.R.    0,5    <L.R.   10,9     1     17,4
 MA3   4     11,7    0,1      0,5    <L.R.   13,9     7,4   7,1    6,6    503      0,9    <L.R.   25,8    10,9   19,5
 BC1   7,2   39,2   <L.R.    <L.R.    10,1   67,2    14,7   7,3   152     239     11,4     4      37,1    3,1    54,1
 BC2   3,2   39,4    0,3      1,3     9,4    92,7    20,9          37     561      8,5    36,9    27,3    1,6    105




even more obvious in the case of narrow streets surrounded by high buildings. This actu-
ally characterises the whole Vittorio Emanuele Avenue.

4. Conclusion

    The monitoring data concerning the conservation state of the materials could be eas-
ily linked to the parameters of environmental quality considering the data gathered by the
other research groups of the project.
                                                                                                                         Conservation Science in Cultural Heritage


    The results reported in this paper are, by now, only a small part of a multidisciplinary
research that will be fruitful, provided a great interaction between the different experts
involved in the project.
    As an example, the group interested in environmental monitoring will provide us with
data concerning gaseous pollutants, which is useful to determine the causes of the
degradation process pointed out in the monuments under study. The nature of the
analysed materials that constitute the substrate and on which actual or potential bio-dete-
rioration happens, will be defined for the biologists. The chemical laboratory of the
C.R.P.R. will organize the analysis of materials, using tools that are not available at the
University, such as the RX fluorescence portable, the mercury porosimeter and the cli-
matic room. The Laboratory of Inorganic Material Restoration of the C.R.P.R. shall rep-

                                                                                                                        &$
                                                                                                            resent an important help in a future experimentation stage as far as the techniques of sur-
                                                                                                            face cleaning and the application of consolidating and protective products are concerned.
                                                                                                               The ambitious and long term object of the SALVALARTE Respira Pulito project is to
                                                                                                            define the “threshold of environmental risks” for the cultural heritage and to assess the
                                                                                                            minimal frequency for a correct “periodical maintenance” of the monument, aimed at
                                                                                                            avoiding restoration thanks to techniques and materials that are appropriate for a better
                                                                                                            and more efficient conservation.
                                                                                                               The choice for the reference sampling sites appeared of utmost importance, even for
                                                                                                            cases different from the situation in Vittorio Emanuele Avenue in Palermo that bears a
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                            high traffic flow. The Walls Timoleontine of Gela (CL) were considered as a particular
                                                                                                            example, insofar as they are exposed to a coast environment polluted by chemical indus-
                                                                                                            tries. Besides, the archaeological area of Morgantina (EN) was also taken into account
                                                                                                            as an example of agricultural area, defined as “white area” because of the lack of pollu-
                                                                                                            tion: it presents us with the case of “natural” degradation of construction materials.

                                                                                                            Thanks

                                                                                                               We thanks the Centro Regionale per il Restauro of the Assessorato ai Beni Culturali
                                                                                                            of the Sicily Region for the help given to the research.

                                                                                                            Bibliography
                                                                                                            [1] LORUSSO S. 2002, La diagnostica per il controllo del sistema manufatto ambiente,
                                                                                                                Bologna, Pitagora Editrice.
                                                                                                            [2] LAURENZI TABASSO M., MARABELLI M. 1994, Il degrado dei monumenti in Roma
                                                                                                                in rapporto all’inquinamento atmosferico, Viterbo, BetaGamma.
                                                                                                            [3] BARBARO S., CARACAUSI R., CHISESI R.M. 2004, Il progetto SALVALARTE respi-
                                                                                                                 ra pulito: uno strumento operativo multidisciplinare per la conservazione e la fruizio-
                                                                                                                 ne dei Beni Culturali nella regione Sicilia, Quaderni di Scienza della Conservazione
                                                                                                                 4/2004, Bologna, Pitagora Editrice, 63-90.
                                                                                                            [4] MELI G., LORUSSO S. 2004, Progetto di ricerca: “Stesura di una carta del rischio
                                                                                                                per la conservazione dei beni culturali negli ambienti confinati”, Quaderni di Scienza
                                                                                                                della Conservazione 4/2004, Bologna, Pitagora Editrice, 43-62.
                                                                                                            [5] AMOROSO G.G. 1995, Il restauro della pietra nell’architettura monumentale,
                                                                                                                Palermo, Flaccovio.
                                                                                                            [6] ALAIMO R. 1989, Caratteristiche composizionali del particolato solido atmosferico e
                                                                                                                chimismo delle acque di precipitazione nell’area urbana di Palermo in F. ZEZZA (ed.),
                                                                                                                La Conservazione dei Monumenti nel Bacino del Mediterraneo, Atti del Convegno,
                                                                                                                Bari, 369-377.
                                                                                                            [7] ERCOLI L., D’AGOSTINO F., RIZZO G. 2003, Le calcareniti e le malte della Porta

                                                                                                       &,
    Nuova di Palermo, in C. D’AMICO (ed), Archeometria del Costruito. L’Edificato
    Storico: Materiali, Strutture e Rischio Sismico, Atti del Convegno, Ravello.
[8] RIZZO G. et al. 2001, Le pietre: caratterizzazione del materiale e stato di conserva-
    zione in G. ALESSANDRINI (ed.), Il Centro Storico di Palermo. La conoscenza per
    la manutenzione, Consiglio Nazionale delle Ricerche, Istituto Nazionale di
    Coordinamento Beni Culturali, Roma, 198-374.




                      VALUTAZIONE DELLO STATO DI CONSERVAZIONE
                      DEI MATERIALI LAPIDEI IN RELAZIONE AL GRADO
                      DI AGGRESSIVITÀ DELL’AMBIENTE NEL QUALE
                      SONO POSTI IN OPERA


                      1. Introduzione
                          Le condizioni di esposizione ambientale dei beni culturali architettonici, con-
                      centrati in larga misura nelle aree urbane, sono divenute negli ultimi decenni
                      progressivamente più aggressive, provocando conseguentemente un’accelera-
                      zione dei processi di degrado e compromettendo talvolta in breve tempo i risul-
                      tati degli interventi di conservazione delle superfici [1-2]. Una delle cause prin-
                      cipali può essere individuata nell’aumento incontrollato del traffico veicolare,
                      per il quale non sembrano esistere possibilità di limitazioni, neppure a garanzia,
                      se non della protezione dei monumenti, almeno della salute dei cittadini che
                      vivono nei centri urbani. Tuttavia la normativa vigente a tutela della salute pub-
                      blica indica dei limiti di concentrazione degli inquinanti atmosferici, superati i
                      quali le amministrazioni comunali devono intervenire per ripristinare condizioni
                      di sicurezza. Un approccio simile sarebbe auspicabile anche per la conserva-
                      zione dei monumenti, con una quantificazione del rischio relativo ai problemi
                      dell’inquinamento che serva ad orientare interventi sia legislativi sia operativi,
                      capaci di ridurre i componenti aggressivi presenti in aree ad elevato contenuto
                      storico-artistico, quale per esempio il centro storico di Palermo.
                          Con questo ambizioso obiettivo di lungo termine si è avviato recentemente
                      in Sicilia il progetto SALVALARTE Respira Pulito, promosso dall’Agenzia
                      Regionale per la Protezione Ambientale (A.R.P.A.), dal Centro Regionale per la
                      Progettazione e il Restauro (C.R.P.R.) dell’Assessorato Beni Culturali della
                                                                                                                 Conservation Science in Cultural Heritage

                      Regione Sicilia, da Legambiente e da alcuni Dipartimenti delle tre Università
                      siciliane. Si tratta di un progetto di ricerca multidisciplinare [3], che prevede in
                      una prima fase la raccolta di dati sullo stato di conservazione dei beni culturali
                      in Sicilia, contribuendo così alla definizione di una “Carta del Rischio dei Beni
                      Culturali”, già in fase di elaborazione da parte del C.R.P.R., anche per ciò che
                      riguarda la conservazione negli ambienti confinati [4]. Uno degli aspetti qualifi-
                      canti della ricerca, legato all’ampio spettro di competenze dei soggetti coinvol-
                      ti, è quello di valutare da una parte le diverse cause del degrado, da quelle chi-
                      miche a quelle fisiche o biologiche, e dall’altra di misurare i più significativi para-
                      metri chimico-fisici ambientali con i quali porre in relazione lo stato di conser-
                      vazione dei monumenti [5-6].
                          Nella prima parte della ricerca si è operato a Palermo lungo l’asse viario di
                      Corso Vittorio Emanuele, che attraversa tutto il centro storico della città da
                      monte fino al mare ed è sottoposto ad un traffico veicolare particolarmente
                      intenso. Il contributo del Laboratorio di Ingegneria Chimica per i Beni Culturali
                      dell’Università di Palermo si articola nelle seguenti fasi:
                      – analisi per la caratterizzazione dei materiali costitutivi più ricorrenti nei manu-
                          fatti di interesse storico-artistico (pietre da costruzione e da rivestimento,
                          intonaci, stucchi, legno strutturale e non, laterizi, etc.);

                                                                                                                &"
                                                                                                       – misura dei parametri chimico-fisici che definiscono il loro stato di conserva-
                                                                                                         zione;
                                                                                                       – analisi dei campioni di particellato atmosferico raccolti dall’Azienda
                                                                                                         Municipalizzata di Igiene Ambientale (A.M.I.A.) e dall’Agenzia Regionale per
                                                                                                         la Protezione Ambientale (ARPA Sicilia);
                                                                                                       – analisi delle cause e dei meccanismi dei processi di alterazione e di degra-
                                                                                                         do dei materiali e correlazione con le condizioni di esposizione, definite attra-
                                                                                                         verso il monitoraggio ambientale effettuato dagli altri gruppi di lavoro.
                                                                                                         In questo lavoro vengono presentati i risultati relativi ad una prima campa-
                                                                                                       gna di campionamento concordata con gli altri Enti che partecipano al progetto.
                                                                                                       2. Materiali e tecniche sperimentali
                                                                                                           I manufatti oggetto di questo studio sono le due porte monumentali che chiu-
                                                                                                       dono l’asse viario di Corso Vittorio Emanuele – la Porta Nuova lato monte, la
                                                                                                       Porta Felice lato mare – e la Biblioteca Centrale della Regione Siciliana, che
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                       prospetta sul corso in una posizione intermedia.
                                                                                                           Per ogni edificio è stato effettuata una campagna fotografica delle tipologie
                                                                                                       di degrado riscontrate. Per ciascun campione prelevato è stata compilata una
                                                                                                       scheda, che riporta la foto e la descrizione dell’area del prelievo. Dove non è
                                                                                                       stato possibile prelevare campioni ci si è limitati a descrivere i fenomeni di
                                                                                                       degrado rilevabili all’osservazione diretta.
                                                                                                           La tipologia dei materiali prelevati comprende lapidei naturali, malte, croste,
                                                                                                       depositi superficiali ed efflorescenze saline. Il campionamento è avvenuto sem-
                                                                                                       pre con tecniche poco invasive, prelevando il materiale da zone nascoste o
                                                                                                       poco accessibili e avendo cura di privilegiare le aree prossime ai punti di moni-
                                                                                                       toraggio scelti dagli altri gruppi. Inoltre sono stati analizzati numerosi campioni
                                                                                                       di particellato atmosferico, la cui composizione in termini di specie cristalline,
                                                                                                       metalli pesanti e sali solubili, può influenzare fortemente la durabilità dei mate-
                                                                                                       riali lapidei. I campioni di particellato provengono da varie centraline
                                                                                                       dell’A.M.I.A., l’ente che ha il compito istituzionale di raccogliere il particellato e
                                                                                                       quantificarne la presenza nell’aria, e da due campagne di monitoraggio della
                                                                                                       qualità dell’aria effettuate dall’ARPA Sicilia alla Biblioteca Centrale e al Museo
                                                                                                       Archeologico Regionale A. Salinas. Le polveri raccolte sono poi state analizza-
                                                                                                       te a cura del Laboratorio di Ingegneria Chimica per i Beni Culturali, anche in col-
                                                                                                       laborazione con il Dipartimento Provinciale (DiP) di Palermo dell’ARPA Sicilia.
                                                                                                           Oltre all’osservazione dei campioni in microscopia ottica, le tecniche analiti-
                                                                                                       che adottate sono la diffrattometria dei raggi X (XRD), la cromatografia ionica
                                                                                                       (IC), la spettrofotometria di emissione con sorgente a plasma-spettrometria di
                                                                                                       massa ICP-MS condotta presso il DiP dell’ARPA.
                                                                                                       3. Risultati e discussione
                                                                                                            Nelle tabelle riportate di seguito i risultati analitici sono raggruppati per pro-
                                                                                                       venienza del campione e per tipologia di analisi. Sia per la Biblioteca Centrale
                                                                                                       della Regione Siciliana che per la Porta Felice sono stati analizzati dieci cam-
                                                                                                       pioni costituiti da croste, malte ed efflorescenze saline (tab. 1-3). Per quanto
                                                                                                       riguarda la Porta Nuova, in occasione di un intervento di restauro nel 2000, era
                                                                                                       stata effettuata una estesa campagna di campionamenti su entrambi i prospet-
                                                                                                       ti, i cui risultati sono stati oggetto di una pubblicazione [7]. Qui vengono ripor-
                                                                                                       tate per confronto solamente le caratteristiche di due campioni prelevati nel-
                                                                                                       l’ambito del progetto SALVALARTE Respira Pulito (tab. 4-5).
                                                                                                            I risultati delle analisi XRD riportati in tab. 2 mostrano che il gesso è presente
                                                                                                       soltanto nei campioni indicati come “croste”. L’origine del gesso può essere
                                                                                                       ricondotta a processi di solfatazione di substrati carbonatici, marmi e calcareni-
                                                                                                       ti ad esempio, ma anche malte a base di calce. Tuttavia le analisi XRD riporta-
                                                                                                       te in tab. 6 rivelano la presenza di gesso anche nel particellato atmosferico,
                                                                                                       come conseguenza del trascinamento eolico da terreni gessosi. Pertanto alcu-
                                                                                                       ni dei campioni indicati come “croste” potrebbero in realtà essere il risultato del
                                                                                                       consolidamento di un deposito di particellato sulle superfici lapidee. Questo
                                                                                                       aspetto dello stato di conservazione degli edifici sarà approfondito con il contri-


                                                                                            )%
buto delle unità operative che nel Progetto SALVALARTE Respira Pulito hanno
il compito di rilevare i componenti gassosi dell’atmosfera urbana, e in particola-
re SO2.
     Inoltre, la presenza di discrete quantità di sodio e magnesio da una parte e
cloruri e solfati dall’altra, mostrata nelle tab. 3 e 5, rivela il ruolo di primaria
importanza dello spray marino nel determinare la presenza diffusa di efflore-
scenze saline.
     Il compito del Laboratorio di Ingegneria Chimica per i Beni Culturali nel pro-
getto complessivo è incentrato sullo stato di conservazione dei materiali, tutta-
via nell’ottica multidisciplinare adottata si è ritenuto utile integrare i dati di altre
unità operative, relativi agli apporti di materiale dall’esterno e alla presenza di
composti aggressivi nell’atmosfera, con un’analisi del particellato atmosferico
mediante le stesse tecniche qui utilizzate per i materiali costitutivi degli edifici.
     I campioni di particellato raccolti dall’A.M.I.A. provengono da tre centraline,
una sita al termine dell’asse viario di corso Vittorio Emanuele, precisamente in
Piazza Indipendenza (I) in prossimità della Porta Nuova, una in Piazza Giulio
Cesare (G), vicino alla stazione centrale di Palermo, sito ad altissima incidenza
di traffico veicolare, ed infine la terza in un’area suburbana di Palermo,
Boccadifalco (F), zona a bassa intensità di traffico veicolare. Nella classifica-
zione dei campioni sono stati considerati anche altri due parametri di grande
rilievo per la loro incidenza sul particellato atmosferico, ovvero la presenza di
precipitazioni piovose e i periodi di accensione del riscaldamento. I campioni
vengono quindi identificati da una prima lettera che indica la centralina di pro-
venienza, una seconda che indica la presenza o meno di riscaldamento, R per
riscaldamento e N senza riscaldamento, una terza per indicare se il campione
è stato raccolto in periodo piovoso (P) o secco (S), ed infine un numero pro-
gressivo per distinguere campioni successivi di uguale provenienza. Ad esem-
pio, quindi, il campione GRP1 è il primo campione (1) prelevato alla stazione
Giulio Cesare (G), in periodo di riscaldamento (R) e piovoso (P).
     I risultati delle analisi XRD, LC e ICP-MS vengono riportati nelle tab. 7-9.
     La presenza di rilevanti quantità di calcite e gesso nel particellato, eviden-
ziata dalle analisi XRD in tab. 6, può essere alla base dei fenomeni di consoli-
damento del deposito superficiale, risultato dei processi di solubilizzazione e
ricristallizzazione conseguenti ai normali cicli di umidità ambientale: questa
considerazione era già emersa nel corso della ricerca effettuata in collabora-
zione con il Centro Gino Bozza del Consiglio Nazionale delle Ricerche di Milano
per conto del Comune di Palermo [8].
     Un confronto tra i risultati delle analisi sui filtri dell’A.M.I.A. e su quelli
dell’ARPA evidenzia una particolare criticità della Biblioteca Centrale, che pro-
spetta sullo stretto asse viario di Corso Vittorio Emanuele, rispetto a quanto rile-
                                                                                               Conservation Science in Cultural Heritage

vato in due piazze non lontane e ad alta intensità di traffico veicolare, Piazza
Giulio Cesare e Piazza Indipendenza. In particolare la concentrazione di macro
elementi dei campioni BC di tab. 9 risulta in molti casi superiore anche di un
ordine di grandezza a quella dei campioni G e I di tab. 8. Ciò indica la presen-
za di una maggiore quantità di particellato atmosferico in prossimità della
Biblioteca, probabilmente come conseguenza del cosiddetto “effetto canyon”,
cioè dell’intrappolamento degli inquinanti emessi, specie dagli autoveicoli e
quindi a bassa quota, in ambiente urbano, fenomeno tanto più evidente quan-
to più le strade sono strette e circondate da edifici alti: situazione che caratte-
rizza il corso Vittorio Emanuele in tutta la sua estensione.
4. Conclusioni
    I dati del monitoraggio sullo stato di conservazione dei materiali possono
essere posti in relazione in maniera significativa con i parametri di qualità del-
l’ambiente solo disponendo di tutti i dati rilevati dalle altre unità operative del
progetto.
    Dunque i risultati qui riportati costituiscono per il momento uno dei contribu-
ti ad un lavoro di gruppo che si articolerà attraverso la massima interazione tra
le diverse professionalità coinvolte nel progetto.


                                                                                           )
                                                                                                                                       Ad esempio il gruppo interessato al monitoraggio ambientale dovrà fornire i
                                                                                                                                   dati sugli inquinanti gassosi, utili per individuare le cause dei processi di degra-
                                                                                                                                   do rilevati nei monumenti studiati. Ai biologi potranno essere forniti i dati relati-
                                                                                                                                   vi alla natura dei materiali analizzati, che costituiscono il substrato sul quale si
                                                                                                                                   sviluppano i processi di biodeterioramento in atto o potenziali. Il Laboratorio
                                                                                                                                   Chimico del C.R.P.R. potrà integrare il lavoro di analisi dei materiali, utilizzando
                                                                                                                                   apparecchiature non disponibili presso l’Università, quali ad esempio la fluore-
                                                                                                                                   scenza RX portatile, il porosimetro a mercurio e la camera climatica. Il
                                                                                                                                   Laboratorio di Restauro dei Materiali Inorganici del C.R.P.R. fornirà un suppor-
                                                                                                                                   to prezioso in una successiva fase di sperimentazione relativa alle tecniche di
                                                                                                                                   pulitura delle superfici e alla applicazione di prodotti consolidanti e protettivi.
                                                                                                                                       L’obiettivo ambizioso e a lungo termine del progetto SALVALARTE Respira
                                                                                                                                   Pulito sarà quello di definire le “soglie di rischio ambientale” per il patrimonio dei
                                                                                                                                   beni culturali e di valutare la cadenza minima per una corretta “manutenzione
                                                                                                                                   periodica” del manufatto, che consenta di prevenire il restauro, individuando le
G' Rizzo et al' ( Assesment of the conservation state of stone materials in relation to the level'''




                                                                                                                                   tecniche e i materiali più idonei per operare gli interventi di conservazione.
                                                                                                                                       In quest’ottica si è ritenuto essenziale individuare dei siti di campionamento
                                                                                                                                   da utilizzare come riferimento anche per situazioni significativamente diverse
                                                                                                                                   dall’asse viario di Corso Vittorio Emanuele a Palermo, che è rappresentativo di
                                                                                                                                   un contesto urbano a forte flusso veicolare. In particolare sono state individua-
                                                                                                                                   te le Mura Timoleontine di Gela (CL), esposte ad un ambiente di tipo costiero,
                                                                                                                                   inquinato dalla presenza di industrie chimiche, e l’area archeologica di
                                                                                                                                   Morgantina (EN), quale area di carattere agricolo, che possa fungere da “bian-
                                                                                                                                   co”, cioè da zona priva di inquinamento cui fare riferimento per il degrado “natu-
                                                                                                                                   rale” dei materiali da costruzione.
                                                                                                                                   Ringraziamenti
                                                                                                                                      Si ringrazia il Centro Regionale per la Progettazione e il Restauro
                                                                                                                                   dell’Assessorato ai Beni Culturali della Regione Sicilia per il supporto fornito alla
                                                                                                                                   ricerca.




                                                                                                        Summary
                                                                                                        The multidisciplinary project SALVALARTE Respira Pulito has been carried out by different research
                                                                                                        groups operating in Sicily. The aim of the project is the assessment of “health risks” for monuments
                                                                                                        in relation to environmental pollution in terms of threshold for the concentration of aggressive com-
                                                                                                        ponents.
                                                                                                        In this framework, the duty of the Laboratory of Chemical Engineering for Cultural Heritage,
                                                                                                        University of Palermo, is to analyse samples taken from monuments in Sicily, in order both to char-
                                                                                                        acterize the constitutive materials and to assess the conservation state. The analytical results are
                                                                                                        related to the environmental conditions monitored by other research groups.


                                                                                                        Riassunto
                                                                                                        Il progetto multidisciplinare SALVALARTE Respira Pulito, promosso da diversi gruppi di ricerca sul
                                                                                                        territorio della Regione Sicilia, ha come obiettivo finale una quantificazione del rischio relativo ai pro-
                                                                                                        blemi dell’inquinamento, che serva ad orientare interventi, sia legislativi sia operativi, capaci di ridur-
                                                                                                        re i componenti aggressivi presenti in aree ad elevato contenuto storico-artistico.
                                                                                                        In questo ambito il Laboratorio di Ingegneria Chimica per i Beni Culturali dell’Università di Palermo
                                                                                                        ha effettuato le analisi per la caratterizzazione dei materiali costitutivi di alcuni manufatti di interes-
                                                                                                        se storico-artistico e la misura dei parametri chimico-fisici che definiscono il loro stato di conserva-
                                                                                                        zione. La finalità del lavoro è quella di analizzare le cause e i meccanismi dei processi di alterazio-
                                                                                                        ne e di degrado dei materiali e di correlarli con le condizioni di esposizione, definite attraverso il
                                                                                                        monitoraggio ambientale effettuato dagli altri gruppi di lavoro.

                                                                                                   )!
Résumé
Le projet multidisciplinaire SALVALARTE Respira Pulito a été mené par différents groupes de
recherché en Sicile. Le but du projet est l’évaluation des “risques” pour la santé des monuments en
relation avec le degré de pollution environnementale en terme de seuil de concentration de compo-
sants agressifs. Dans ce cadre, le travail du Laboratoire d’Ingénierie chimique pour le patrimoine cul-
turel, Université de Palerme, est l’analyse des échantillons relevés dans des monuments en Sicile,
afin de pouvoir définir les matériaux constituants et évaluer l’état de conservation. Les résultats d’a-
nalyse sont intrinsèquement liés aux conditions environnementales étudiées par d’autres groupes
de recherche.


Zusammenfassung
Das multidisziplinären Projekt SALVALARTE Respira Pulito wurde von einigen Forschungsgruppen
gefördert, die in Sizilien arbeiten. Ziel des Projektes ist die Evaluation der “Gesundheitsgefährdung”
für Denkmäler, verbunden mit der Umweltverschmutzung, um legislative und operative
Entscheidungen zu beeinflussen.
In diesem Rahmen ist es die Aufgabe des Laboratory of Chemical Engineering for Cultural Heritage,
Universität von Palermo, die Proben aus sizilianischen Denkmälern zu analysieren, um die konsit-
vien Materialien zu analysieren und den Konservierungszustand zu evaluieren.
Die analytischen Resultaten sind gebunden an die Umweltkonditionen, überwacht von anderen
Forschungsgruppen.


Resumen
El proyecto multidisciplinar SALVALARTE Resprira Pulito, promovido por diferentes grupos de
investigación en el territorio de Sicilia, tiene como objetivo final la cuantificación del riesgo relacio-
nado con los problemas de la contaminación, para que puedan orientar las intervenciones, tanto
legislativas como operativas, capaces de reducir los componentes agresivos presentes en áreas de
elevado contenido histórico-artístico.
En este ámbito el Laboratorio de Ingeniería Química para los Bienes Culturales de la Universidad
de Palermo ha realizado los análisis para la caracterización de los materiales constitutivos de unas
obras de interés histórico-artístico y la medida de los parámetros químico-físicos que definen su
estado de conservación. La finalidad del trabajo es analizar las causas y los mecanismos de los pro-
cesos de alteración y degradación de los materiales y dotarlos de las condiciones de exposición,
definidas a través de la vigilancia ambiental realizada por otros grupos de trabajo.
                                                                                                              Conservation Science in Cultural Heritage




                                                                                                             )&
